CHEMICAL ADMIXTURES FOR CONCRETE PAVING MIXTURES
APRIL 2019 FHWA-HIF-18-017
Hydraulic cement concrete (hereafter referred to simply as concrete) is composed of
aggregates bound together by a hydrated cement paste. Concrete is readily
available, affordable, and is known for its longevity. Fresh concrete used in paving
must possess the workability to be mixed, transported, placed, consolidated, and
finished to a homogenous condition using the means and methods dictated by
specification and the given project constraints. Concrete paving often entails
placement with a slipform paver, which requires a mixture that readily consolidates
under vibration but resists edge sloughing once the paver sideforms pass. The
hardened concrete must possess the required physical properties needed to achieve
design expectations while also exhibiting adequate durability characteristics over the
service life. To achieve these fresh and hardened concrete properties, it is often
necessary to use chemical admixtures.
The proper use of chemical admixtures requires the following (Kosmatka and Wilson
• Adherence to manufacturer’s information to confirm that the admixture under
consideration is appropriate for the proposed application.
• Following the manufacturer’s recommendations regarding admixture dosage
and establish the optimum dosage through laboratory testing.
• Trial batching with the admixture and other job-mix concrete constituents under
temperature conditions that are expected to exist at time of placement to assess
the potential for interactions on fresh and hardened concrete properties.
Whether using a single admixture or a combination of many admixtures, their use
provides an additional means of controlling the quality of concrete by modifying one
or more mixture properties in a beneficial way. However, admixtures must not be
used in an attempt to correct for poor-quality materials, improper proportioning of the
concrete, and/or inappropriate placement procedures (ACI 2012).
It is important that the cost effectiveness of the admixture not be judged on the
increase in cost to the concrete alone, but instead on the overall cost of the concrete
in place as the proper use of chemical admixtures can provide significant savings
with regards to transporting, placing, and finishing concrete (ACI 2016b). In addition,
the performance of the concrete in service must be considered as admixtures can
significantly improve longevity at little additional cost (e.g., enhance freeze-thaw
resistance due to entraining air). A number of excellent resources exist that provide
detailed information on chemical admixtures (ACI 2012; ACI 2016b; Kosmatka and
This Tech Brief focuses on enhancing the fresh and/or hardened properties of paving
grade concrete through the use of chemical admixtures. The chemical admixtures
most commonly used in paving concrete are discussed in detail, specifically those
used to entrain air, reduce water, and modify set. Other admixtures that are
occasionally used in paving concrete are also introduced, including those for
hydration control, shrinkage reduction, inhibition of the alkali-silica reaction (ASR),
and for coloration.
The images above are Applied Pavement Technology originals
and FHWA has permission to utilize them in this Tech Brief.
2 Chemical Admixtures for Concrete Paving Mixtures
AIR ENTRAINING ADMIXTURES
As concrete freezes, ice first forms within the larger pores.
The formation of ice is expansive and results in changes
in the pore solution chemistry, together resulting in the
generation of stress within the concrete (Powers 1945;
Powers 1954; Powers 1955; Powers and Helmuth 1956;
Marchand, Pleau, and Gagné 1995; Penttala 1998;
Scherer and Valenza 2005). The presence of a network
of uniformly dispersed entrained air bubbles (such as
shown in figure 1) can provide the needed empty space
to relieve stress generated as the concrete freezes. A
more thorough discussion on protecting concrete against
freeze-thaw damage can be found in ACI (2016a),
Kosmatka and Wilson (2016), in the commentary to
AASHTO PP 84-17, and in a recent FHWA Tech Brief
(Van Dam 2019).
Figure 1. Stereo micrograph of entrained air voids
(spherical bubbles) in hardened concrete. Larger,
irregular voids are entrapped air.
© 2019 Karl Peterson
Mechanisms for Air Entrainment
Air is most commonly entrained in concrete during
batching through the addition of an air-entraining
admixture (AEA) specified in AASHTO M 154 (ASTM
C260). The most common AEAs are composed of salts
of wood resins (e.g., Vinsol resin), organic salts of
sulfonated hydrocarbons, fatty and resinous acids and
their salts, salts of proteinaceous acids, and/or synthetic
detergents (ACI 2016b; Kosmatka and Wilson 2016).
AEAs are surfactants that work at the air-water interface
to create stable air bubbles in the fresh concrete as it is
mixed. These bubbles remain once the concrete has
hardened and, ideally, are uniformly dispersed throughout
the mortar phase in the concrete. The stiffness of the
concrete mixture, the type and duration of mixing,
temperature, and many other factors are influential in the
formation of the entrained air. Excellent summaries of
these factors are provided by Nagi et al. (2007) and by
Kosmatka and Wilson (2016).
Air Content Requirements
The air content required to protect concrete is dependent
on both the freeze-thaw exposure condition and the paste
content (or mortar fraction) in the concrete (ACI 2016a).
For most paving mixtures exposed to freezing and
thawing and where deicers are used, the recommended
air content should be between 5.0 and 8.0 percent or
greater than 4 percent with a Super Air Meter (SAM)
number less than 0.20 measured in accordance with
AASHTO TP 118 (AASHTO PP 84-17).
Properties of Air-Entrained Concrete
The principal reason to entrain air in concrete is to protect
the concrete against damage from freezing and thawing.
But air entrainment has other impacts on concrete, both
positive and negative.
With regards to fresh concrete, entrained air improves
workability, making the concrete more cohesive and
allowing for significant reductions in water and sand
content. Further, the tendency for segregation and
bleeding is reduced and finishing qualities improved
(Kosmatka and Wilson 2016). Although a reduction in
bleeding can have positive impacts, one potential
negative is that in highly evaporative environments (hot,
windy, and/or dry), the risk of plastic shrinkage cracking
is increased as bleeding is diminished (ACI 2016b).
With regards to hardened concrete, the addition of air
reduces concrete strength, with a 1 percent increase in air
commonly equated to a 5 to 6 percent reduction in
strength (Kosmatka and Wilson 2016). Yet the
improvement in workability allows for a reduction in water
that can be used to reduce the water-to-cementitious
materials ratio (w/cm) in air entrained concrete. This can
compensate for the loss in strength due to the increased
air (ACI 2016b).
Troubleshooting Air Entrainment Problems
In most cases, the total air content of the fresh concrete
prior to placement is correlated with and similar to the total
air content in the hardened concrete. Further, the total air
content is usually a good indicator of the acceptability of
the air-void system in offering protection against freeze-
thaw damage. But this is not always the case as there
are times when the total air content in the fresh concrete
is acceptable prior to placement but an unacceptable air-
void system is present in the hardened concrete. These
problems can be generally classified into the following two
• Air-void system instability results in loss of air through
handling and consolidation.
• An irregular air-void system is produced with regards
to bubble size and spacing.
With regards to air-void system instability, it is common to
lose 1 to 2 percent of the air through the placement
process when the concrete is placed and/or consolidated
3 Chemical Admixtures for Concrete Paving Mixtures
(Whiting and Nagi 1998; Taylor et al. 2007; Ram et al.
2012). It is generally thought that the air that is lost is in
the larger air bubbles, and those larger bubbles are not
as critical to freeze-thaw protection as the smaller
bubbles. But air loss beyond this is of concern, and may
be a result of a number of other factors including AEA
interactions with other chemical admixtures having a
negative effect on air void stability (Nagi et al. 2007).
Organic impurities may also decrease the effectiveness
of AEAs. This is of particular concern with regards to fly
ash, in which carbon present due to incomplete coal
combustion, or worse yet, activated carbon added to
mitigate mercury emissions, can significantly destabilize
Assessing the air content of fresh concrete over time
provides a good indication of the air-void system stability.
Such testing is common when determining mixture
proportions in the laboratory and should be repeated as
materials change during construction. Furthermore,
periodically testing the air content of the concrete after the
paver will provide a good indication of air loss due to
Another problem is that concrete having acceptable
volumes of air may remain susceptible to freeze-thaw
damage because of an irregular air-void system.
Irregularity may include:
• Large bubbles spaced far apart – This can occur
due to interactions between the AEA and another